Achieving balanced UV SHG responses, optical band gaps and birefringence in rare earth compounds Ln(IO<sub>3</sub>)(SO<sub>4</sub>)·3H<sub>2</sub>O (Ln = Y, Gd, Er, Ho, Dy, Eu).
Ma, Shihua; Geng, Lei; Zhu, Baozhu; Meng, Changyu; Dalton transactions (Cambridge, England : 2003) 54 (2025) 8183–8189; doi:10.1039/d5dt00613a

data_7719006
_publ_section_title
;
 Achieving balanced UV SHG responses, optical band gaps and birefringence
 in rare earth compounds
 Ln(IO<sub>3</sub>)(SO<sub>4</sub>)&#xb7;3H<sub>2</sub>O (Ln = Y, Gd, Er,
 Ho, Dy, Eu).
;
_journal_issue                   20
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              8183
_journal_page_last               8189
_journal_paper_doi               10.1039/d5dt00613a
_journal_volume                  54
_journal_year                    2025
_chemical_formula_sum            'H6 I O10 S Y'
_chemical_formula_weight         413.92
_space_group_crystal_system      orthorhombic
_space_group_IT_number           19
_space_group_name_Hall           'P 2ac 2ab'
_space_group_name_H-M_alt        'P 21 21 21'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2025-03-14 deposited with the CCDC.	2025-04-14 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.6961(5)
_cell_length_b                   8.7941(8)
_cell_length_c                   13.6473(11)
_cell_measurement_reflns_used    3553
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.54
_cell_measurement_theta_min      2.76
_cell_volume                     803.64(11)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0174
_diffrn_reflns_av_unetI/netI     0.0242
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.985
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            4129
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.538
_diffrn_reflns_theta_min         2.755
_exptl_absorpt_coefficient_mu    11.394
_exptl_crystal_colour            COLORLESS
_exptl_crystal_density_diffrn    3.421
_exptl_crystal_description       STICK
_exptl_crystal_F_000             776
_refine_diff_density_max         0.451
_refine_diff_density_min         -1.228
_refine_diff_density_rms         0.195
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.590(8)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     137
_refine_ls_number_reflns         1818
_refine_ls_number_restraints     9
_refine_ls_restrained_S_all      1.047
_refine_ls_R_factor_all          0.0186
_refine_ls_R_factor_gt           0.0182
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0302P)^2^+0.5031P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0476
_refine_ls_wR_factor_ref         0.0478
_reflns_Friedel_coverage         0.700
_reflns_Friedel_fraction_full    0.998
_reflns_Friedel_fraction_max     0.996
_reflns_number_gt                1792
_reflns_number_total             1818
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d5dt00613a2.cif
_cod_data_source_block           A
_cod_database_code               7719006
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              28053
_shelx_hkl_checksum              29097